**Chapter IV. Probing the reversible fluoride-ion electrochemical reaction by**

**1. Introduction to X-ray diffraction (XRD) and atomic pair distribution function (PDF)**

**1.3. What is PDF analysis**

The Pair Distribution Function, or PDF in short, also noted G(r), is a real space function giving
the probability of finding pairs of atoms separated by the distance r, in the material[97]. It is a
powerful technique capable to probe both the local (low *r) and intermediate (high r) range *
structure of materials. Unlike Bragg scattering which only gives information about the average
structure, PDF analysis is able to shed light on the local structure of amorphous materials
(glasses and even liquids) and highly disordered crystalline materials (nanomaterials), which is
very useful when investigating electrochemical processes happening in electrode materials[10],
[98], [99]. Indeed, electrochemical conversion tends to create disordered nano-domains which
can be hardly detected by conventional XRD. For instance, in Li batteries using conversion
materials, the metal fluoride MF*x *electrode is converted to nano-domains (a few nm wide) of
the corresponding metal M, embedded in a LiF matrix. These reactions cannot be probed by
conventional diffraction techniques, unlike with PDF analysis. Indeed, PDF takes benefit of the
information contained in the diffuse intensity which contains information about the
discrepancies in the local structure of the analysed material.

From a conceptual point of view, G(r) can be expressed in function of the atom-pair density
function (or microscopic pair density), ฯ(r), and the atomic number density (or average number
density), ฯ*0*, as follow:

๐บ(๐) = 4๐๐[๐(๐) โ ๐_{0}] = 4๐๐๐_{0}[๐(๐) โ 1] 63.

With g(r) the atomic pair distribution function. Consequently, the amplitude of **G****(****r****) will be **
**thus dependent upon the mass number of the considered atoms, their density (i.e. **

**quantity), and the probability of finding them separated by the distance ****r****. **
The PDF obtained can be expressed as follow:

๐บ(๐) =_{๐}^{2}โซ ๐น(๐) sin(๐๐)๐๐_{0}^{โ} 64.

With F(Q) the reduced structure function, which can be expressed in function of the total scattering is the normalized structure function S(Q):

๐น(๐) = ๐[๐(๐) โ 1] 65.

Appendix

In practice, only finite Q values can be reached. The PDF is therefore obtained by a sine Fourier transform of the total scattering structure function with limited Q boundaries:

๐บ(๐) =_{๐}^{2}โซ_{๐}^{๐}^{๐๐๐ฅ}๐[๐(๐) โ 1] sin(๐๐)๐๐

๐๐๐ 66.

S(Q) is obtained from experimental diffraction intensity I(Q) after application of corrections
accounting for sample and instrument contributions. High Q*max* thus yields better resolution in
PDF analysis. In order to illustrate what a PDF looks like and the influence of *Q on the *
resolution of the PDF, Figure 0.1 shows the PDF of LBF with various Q values.

0 2 4 6 8 10 12 14

Q = 5 ร
^{-1}
Q = 8 ร
^{-1}
Q = 20 ร
^{-1}

*G*(*r*)

r (ร )

Q = โ

**Figure 0.1.** PDF of La*0.95**Ba**0.05**F**2.95** calculated for different Q values. *

Using conventional X-rays sources like ฮปCuKฮฑ = 1.5418 ร
, and considering that sinฮธ โค 1, Q โค
4ฯ/ฮธ and thus Q โค 8 ร
^{-1}. Figure 0.2 illustrates well that the amplitude of G(r) is dependent
upon the mass number of the relevant atom.

Appendix

0 2 4 6 8 10 12 14

F-F only La-F only La-La only

*G*(*r*)

*r (ร
)*

All distances

ร 15

**Figure 0.2.** PDF of La*0.95**Ba**0.05**F**2.95 **and the corresponding reduced PDF of the La-La, La-F *
*and F-F distances (Q = โ). The G(r) amplitude for the F-F distances was multiplied by 15 to *

*illustrate the low intensity of the F-F reduced PDF. *

Even if the ratio F/La is around 3 in LBF, the amplitude of the F-F contribution to the PDF is almost not visible when compared to that of the La-La and La-F contributions, due to the large mass of La (138.9 u) compared to that of F (19.0 u).

1.3.1.PDF analysis and HEXRD in practice

Hard X-rays were collected at the 11-ID-B beamline of the Advanced Photon Source of Argonne National Laboratory, USA. The powdered samples were sealed in Kapton capillaries (Cole-Parmerยฎ, polyimide tubing, 0.0435โ outside diameter, 0.0020โ wall) under argon atsmosphere, using epoxy glue.

The PDF analysis results used total scattering data recorded at 58.66 or 86.7 keV, i.e., 0.21140 and 0.1430 ร , with sample to detector distances of 175 and 245 mm, respectively. Such sample to detector distance was employed to obtain high Q-range. The data were recorded using an amorphous silicon-based area detector (PerkinElmer).

Diffraction data were simultaneously recorded with a sample to detector distance of about 945 mm to optimize them for 2ฮธ resolution. The I(Q) data (intensity presented in Q space) could be conveniently converted to I(2ฮธ) classical CuKฮฑ XRD data using the relation:

๐ = ^{4๐ sin ๐} โ 2๐ = 2 arcsin^{๐๐} 67.

Appendix

*1.3.1.1.Conversion of total scattering data to the PDF *

Total scattering data (.chi files) were converted to the PDF using PDFgetX2 software[89].

Various S(Q) optimization/corrections were applied to the total scattering data to obtain quality PDFs. Most of these corrections can be found on the annotated demo (https://www.youtube.com/watch?v=9qarGvEYTvQ) of PDFgetX2 provided by Karena Chapman of the Advanced Photon Source. Many useful videos relevant to PDF analysis, including an introduction to PDFgui (software for the refinement of PDF data), can be found on her youtube channel.

First, the background (empty capillary) contribution was corrected. For the samples containing LBF, some fluorescence coming from LaF3 (K-edge = 39 keV) could be observed, particularly when data were recorded at 58.66 keV. Recording at 86.7 keV helped but did not entirely solve the problem. To palliate this, a large constant (โAdd Sam. Bkgโ) was added to the kapton background contribution. Using the fluorescence S(Q) correction with a constant of the same value provided similar results.

To adequately account for Compton (inelastic) scattering, which is a crucial correction, the weight ratios of each atom present in the analyzed powder was calculated and entered in the sample information page. When discharged products were analyzed, a rough estimation of the ratios was calculated. The intensity of the relative phases observed on the HEXRD patterns helped doing so. A 1/E quadratic energy dependence (a & b factors) was employed to efficiently correct Compton scattering.

Laue diffuse scattering was also accounted. A weighting function type โ<asf>^2โ was used.

Oblique incidence was corrected using a transmission coefficient of 0.2 unless significant deviation at high-Q was observed (i.e. increasing intensity at high-Q). A superior value, up to 0.4 was then used, although the correction did not significantly modify the G(r) yielded.

*1.3.1.2. PDF analysis, refinement of the PDF *

The refinement of the PDF was performed using PDFgui[90], a graphical user interface (GUI) based on the PDFfit2[100] software used for the full-profile fitting of PDF data by least square refinement.

In a typical fit, PDF data obtained from PDFgetX2 (.gr files) are refined using one or multiple phases. Each phase contains a set of parameters (lattice parameters and angles, atoms etc.) that can be constrained for refinement. In all of the PDF refinements exhibited in this manuscript,

Appendix

๏ท Lattice parameters *a, b, c, with a same constraint for similar values (e.g. a single *
constraint for cubic systems)

๏ท *scale factor (related to the ratio of the concerned phase and scale of the PDF data) *

๏ท *delta2 (quadratic atom correlation factor, peak sharpening), *

๏ท *sratio (low r peak sharpening), only if delta2 is not employed, with a rcut fixed right *
after the 1^{st} interatomic distance

๏ท *spdiameter (crystallite size), only if relevant, *

๏ท isotropic atomic displacement factors (ADPs) u11, u22, u33, with an identical constraint for similar atoms (e.g. same constraint for all La atoms, another for all F atoms, etc.) For more details about the parameters, please refer to the PDFgui manual/user guide (http://www.diffpy.org/doc/pdfgui/pdfgui.pdf).

Unacceptably high ADPs (> 0.04) were usually due to low scale factors (< 0.02), generally meaning that the weight ratio of the concerned phase was below 1 %. In this case, a value of 0.008 was fixed for cations and 0.01 for anions and no further refinement on ADPs was performed until the scale factor was sufficiently high.

For multiphased refinements, the lattice parameters were carefully refined. Once again, when the weight ratio of the concerned phased was very low, refinement of the lattice parameters usually lead to unlikely values. For instance, a refined value of 6.60 ร for a starting value of 5.56 ร was deemed unacceptable, especially when no significant 2ฮธ deviation was observed on the XRD patterns. When deviation was deemed too large, the lattice parameters were fixed to values taken from literature or from a previous single-phase refinement that yielded reproducible values.

The data set also contains some parameters than can be refined, especially the Q dampening factor (Qdamp). Its value depends on the instrument (Qresolution) and is characterized by a loss of amplitude of G(r) at high r. In our case, refinement leads to values of 0.04 to 0.05. The value of Qdamp was set to 0.045 for all refinements for comparative purposes.

The quality of the refinement is characterized by the weighted R-value noted R*w*. The R-value
describes the difference between the experimental observation (data) and the calculated value
(fit) for a single data point. The R*w* is the R-value weighted for data points i, and is given by the
formula:

Appendix

๐
_{๐ค} = โ^{โ}^{๐}^{๐=1}^{๐ค(๐}_{โ}^{๐}^{)[๐บ}_{๐ค(๐}^{๐๐๐ }^{(๐}^{๐}^{)โ๐บ}^{๐๐๐๐}^{(๐}^{๐}^{)]ยฒ}

๐)๐บ_{๐๐๐ }^{2}

๐๐=1 (๐_{๐}) 68.

With ๐บ_{๐๐๐ } and ๐บ_{๐๐๐๐} the observed (data) and calculated (fit) PDF and ๐ค(๐_{๐}) the weight for each
data point.

The R*w* value under which the refinement can be considered good is subjective and dependant
on the number of phase entering in consideration, but we can consider that values *R**w* > 0.2
indicate a bad refinement. For a single phase, well crystallized material with little defects, a R*w *

< 0.1 can even be expected. For a multiphased, nanocrystalline material, R*w *< 0.1 are almost
impossible to reach.

In general, 0.10 < R*w *< 0.15 suggest that the phase(s) considered are in good agreement with
the observed PDF and that the refinement is sufficiently good.

It is worth noticing that PDFgui also gives the difference curve between the observed and calculated curves. A specific pattern in the difference curve can be revealing of an additional phase present in the material and careful consideration should be brought upon it.

Finally, it is crucial to remember that both XRD and PDF analysis are complementary.

Determining by XRD the crystalline phases present in the material before carrying out PDF analysis is a necessity. Inversely, characterizing nanocrystalline/amorphized materials, or phases present in small amounts, will be impossible without PDF analysis.

Appendix